Conducting Polymers1. Introduction 2.4. Poly(phenylene)s 2.5. Poly(phenylene vinylene)s2. Electron-conducting polymers 2.6. Oligomers 2.7. Ladderpolymers2.1. Poly(acetylene)s 2.8. Poly(thiophene)s2.2. Theory of Conductivity 2.9. Poly(pyrrole)s2.2.1. Conduction mechanism 2.9.1. Stille Coupling2.3. Poly(diacetylene)s 2.10. Poly(aniline)sOne can distinguish between three types of conducting polymers:• Electron-conducting polymers• Proton-conducting polymers• Ion-conducting polymersEach polymer type has already found widespread use in many, mainly optical and electronic applications such as batteries,displays, plastic wires, optical signal processing, information storage, solar energy conversion, etc.. Although conductingpolymers have been known for at least 25 years (reports on the synthesis date back to the last century), it was only in the early90s that a tidal wave of renewed and amplified interest in these materials has catalysed many new developments, both on afundamental level as well as from the manufacturing side. In particular the discovery of light-emitting polymers in 1990, inthe Cavendish Laboratory at Cambridge University, was a major if not the turning point in the fortunes of plastronics, i.e. theuse of polymeric materials as substitute for metal and their derivatives in electronic devices. Serious problems like oxidativestability and device lifetimes have to be overcome, but one does not have to be a soothsayer to predict that one day in the notso distant future we will all go to the beach, carrying our table-set sized flexible LED display with us. Solar-powered, we willsit down and read our paper, surf the net or simply be watching TV.This part of the fourth year lecture course will present an overview on the synthetic strategies of synthesising electron-conducting polymers.1. IntroductionPolymers (Plastic) shape our lives because polymers can be shaped! Is it really necessary to point this out? Maybe not, but itis the major driving force behind most research that tries to design plastics fit for electronic applications. Polymers have theadvantage that they are so much more easily to be processed than metals for example. One can very easily cover largesurfaces with a spin-coated polymer solution. Once the solvent has evaporated one is left with a layer of polymer chains.Most plastics can be deformed reversibly and they also do not break easily, which is not true for metals. These properties andthe ease with which polymers can be shaped into complex multi-polymer architectures are the reasons that have enticed manyscientist and industrialist looking for novel applications and new products.The ability to synthesise what we have identified to be the ideal molecular structure is paramount to a successful and fruitfulexploitation of polymers for the sake of plastronics. In the following we will emphasise on synthetic strategies andmethodologies used in the synthesis of conducting polymer rather than covering the almost limitless structural variations thatone can introduce.
2. Electron-conducting Polymers2.1. Poly(acetylene)sThe first conducting polymer synthesised was poly(acetylene). The first reports on acetylene polymers date back to the lastcentury. Cuprene, a highly crosslinked and extremely irregular product of acetylene polymerisation in the presence of copper-containing catalysts being a typical example for the initial efforts. Poly(acetylene) is the simplest conjugated polymer. In itslinear form it precipitates as a black, air sensitive, infusible and intractable powder out of solution and can not be processed.Ant et al. were the first to polymerise acetylene in hexane using a mixed catalyst of alkyl aluminium and titaniumtetraalkoxides:Natta’s route (1958) to poly(acetylene) resulting in intractable, infusible, air sensitive black powders. Al(Et)3 / Ti(OPr)4Shirakawa’s route (1970s; Nobel Prize for Chemistry 2000) to poly(acetylene) yielding polymer films of up to 0.5 cmthickness. The first example of conducting poly(acetylene) upon doping with halogens or AsF5.
Al(Et)3 / Ti(OBun)4 mainly cis -78oC Al/Ti = 3.5-4 film thickness 10-5 - 0.5 cm toluene Al(Et)3 / Ti(OBun)4 -78oC mainly trans Al/Ti = 1 toluene film thickness 10-5 - 0.5 cm n Al(Et)3 / Ti(OBu )4 approx. cis/trans 50/50 -78oC Al/Ti = 3.5-4 silicone oil film thickness 10-5 - 0.5 cmReaction conditions allow to control the morphology of the conjugated polymer obtained as powder, gel, spongy mass or afilm. Iodine doping renders these polymers conducting and values of up to 105 S/cm have been claimed. Films can bestretchedThe inherent insolubility and infusibility of poly(acetylene) coupled with its sensitivity to air imposes a barrier to theprocessability of the polymer. As a result considerable research efforts have been directed towards obtaining processablepoly(acetylene) by means of polymer analogous transformation. Two syntheses are of particular importance.Dehydrohalogenations of poly(vinyl chloride) Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl Cl head to head tail to tailDrawbacks of this route are short conjugation length, structural defects and crosslinks. Thermally convertable prepolymers(Precursor routes) F3 C F3 CF3 C F3 C ROMP n heat n heat Durham RouteProperty advantages of poly(acetylene) prepared by precursor routes:• Continuous solid films with densities of 1.05-1.10.• Controlled morphology range; amorphous, semi-crystalline, crystalline.• Films can be stretched during or prior to conversion
H H H H H H H H H H H H H H H H H H H H H H H H H H H H H H H H insoluble R R R R R R R R R R R R R R R H R H H H H H H H H H H H H H H H soluble short conjugation length H H H R H H H R H H H R H H H hv or heatR H H H H H H H H H H H H H H H n soluble long conjugation length tungsten alkylidene catalystR GrubbsThe conductivity of all substituted poly(acetylene) analogues reported to date is significantly lower than that forpoly(acetylene) itself. The reduction in conjugation length is attributed to steric repulsions between adjacent side groupswhich causes the polymer chains to twist (rotation barrier single bond: 6 kcal/mol). Grubbs showed that monosubstitutedcyclooctatetraenes can be “ROMPed” to give partially substituted poly(acetylene)s) that are both soluble and highlyconjugated.2.2. Theory of ConductivityPoly(acetylene) provides the limiting case of a polyene of infinite conjugation length. The Hückel energy levels for anypolyene with n unsaturated carbon atoms and with equal bond lengths can be obtained by appeal to the Frost mnemonic forlinear polyenes in which a polygon of order 2n+2 is inscribed in a circle of radius 2ß. At the limit of infinite chain length, thisrelationship still holds, except the polygon is a circle itself. Projection of the semicircle containing the equal density of energylevels along the circumference produces an envelope of energy levels commonly referred to as the density of states.Significantly, the HOMO-LUMO energy difference, or band gap, vanishes. Population of the conduction band requires noenergy and thus the system should be metallic.This non-sensical result arises from the error in assumption of equal bond lengths and resonance integrals. A half-occupationof the conduction bands leads to a Jahn-Teller distortion for quasi-one-dimensional systems called the Peierls distortion. Theresult of this is two inequivalent ground states “R” and “L” with alternating bond lengths and a non-zero gap requiringactivation energy for the intervconversion of the two forms and thus forming an insulating material. R form L form
The Peierls distortion corresponds to a thermally forbidden energy level crossing problem in the Woodward-Hoffmann rulesense. The HOMO for a polyene of arbitrary length is characterised by bonding interactions between the “doubly”-bondedcarbon and antibonding interactions between “singly” bonded carbon. The LUMO is analogous, except that anti-bondinginteractions are found between “doubly” bonded carbon and bonding between “singly” bonded carbon.As a result the symmetric HOMO of the “R” form corresponds to the LUMO of the “L” form and vice versa.Let us restate the above in other words: As predicted by theory, the low dimensional structure of a polyene (of equal bondlength and resonance integral) is unstable and the coupling of electrons and phonons with lattice distortions leads to alocalisation of single and double bonds which lifts the degeneracy and results in a localisation of π electrons with the openingof a bandgap (Eg) generally larger than 1.50 eV.The HOMO-LUMO energy gap of a linear conjugated system (∆E) and the Eg value of the resulting material are usuallydetermined from the low energy absorption edge of the electronic absorption spectra. Both values can also be determinedfrom solution oxidation and reduction potentials (CV).2.2.1. Conduction mechanismAgain, poly(acetylene) is taken as an example to illustrate principles of conduction mechanisms in conducting polymers. L form R form solitonAs a necessary consequence of the asymmetry of the poly(acetylene) ground state, two equivalent polyene chains R and L areinterconverted through the intervention of a mobile charge carrier, a soliton. The soliton is a mobile charged or neutral defect,or a “kink” in the poly(acetylene) chain that propagates down the chain and thus reduces the barrier for interconversion.The charge carrier in n-doped (negatively charged) poly(acetylene) is a resonance-stabilised polyenyl anion of approximately29-31 CH units in length, with highest amplitude at the centre of the defect. This description is backed up by chemical shiftsfound in the 13C NMR spectrum, which indicate increased charge density at the centre of such anions. Also advancedtheoretical calculations (MNDO) are in agreement with this description.So how does a soliton manage to travel from one end of a sample to the other? This can be explained by the bipolaronhopping mechanism:Most experimental data is consistent with a rate-limiting interchain charge transport. If short chains are involved, conductionin poly(acetylene) requires some mechanism for transfer of charge from one chain to another (e.g. intersoliton hopping).Current theories for interchain charge transfer centre around the Kivelson “percolation” mechanism. For n-type solitons(Carbanions) this involves electron transfer from the anion to a neutral soliton (radical) in a neighbouring chain in anisoenergetic process. However the lattice distortion associated with interpolaron hopping (hopping between a radical
carbanion and a neutral polyene chain) is thought to present inaccessible energy barriers. A solution to this dilemma isprovided by organic carbanion chemistry. Charge transfer between carbanions often involves a disproportionation equilibriumbetween a neutral/dianion pair (ion triplet) and a radical anion pair. It is recognised that at the moment this mechanism mostclosely matches the charge transport energetics.Bipolarons in poly(p-phenylene) n2.3. Poly(diacetylene)sPoly(diacetylene)s are prepared by the topochemical polymerisation of diacetylenes.2.4. Poly(phenylene)sFour synthetic routes have been employed for the preparation of poly(phenylene)s. Oxidative coupling, organometalliccoupling, dehydrogenation of poly(cyclohexylene)s and cycloaddition reactions.Oxidative coupling AlCl3 / CuCl2 n -e- -e- n -H + / -H n
The structural features (meta or ortho linkages) and physical properties of the polymer prepared by oxidative coupling dependto a large extend on the nature of the oxidising reagent. Ortho linkages can be introduced by using more substituted benzenesrather than the parent compound. Polymers substituted in the para position are in general more difficult to process, i.e. theyare more ordered and thus π stacking is more efficient.Organometallic coupling Cl Mg ClBr Br or Fe(III), Co(II), Ni(II) n catalysisUllmann and Wurtz-Fittig reactions have been utilised for the synthesis of phenylene oligomers but these methods can not beapplied to the synthesis of poly(phenylene)s since yields are low.Dehydrogenation of poly(cycohexylene)s AIBN heat O2, dioxygens enzyme nRCO2 O2CR Pseudomonas putidaDiester derivatives of 5,6-dihydroxy-1,3-cyclohexadiene have been polymerised radically after which the resultingpoly(cyclohexylene)s were converted to poly(phenylene)s by pyrolysis. Best results were obtained with methyl carbonatederivatives. The dihydroxy monomer precursor is accessible through enzymatic oxidation of benzene. An environmentallyfriendly route to conjugated/conducting polymers.Cycloaddition reactions1,4-cycloadditions of bis-cyclopentadienones with bisacetylenes can yield high molecular weight polymers which containapproximately equal amounts of meta and para substituted phenylene units. R R R n n O O O O O O R R R n R R R n n R R R nSuzuki coupling of p-bromophenyl boronic acid offers another convenient route to poly(phenylene) although substitutedanalogues require elaborate syntheses of monomer units. An interesting extension of this methodology is the synthesis ofhyperbranched poly(phenylene)s from an AB2 monomer. In general branching improves solubility and processibilitycompared to the linear parent polymer, which is also true in the case of highly conjugated polymers such as poly(phenylene)s.
Pd(PPh 3)4Br B(OH)2 n Br Br Br Pd(PPh 3)4 B(OH)2 Br Br Br Br Br Br Br Br Br BuLi CO2 Br Br Br Br Br Br Br2.5. Poly(phenylene vinylene)sPoly(phenylene vinylene) (PPV) possess a chemical structure which is intermediate between that of poly(acetylene) andpoly(phenylene). Oriented PPV is highly crystalline, mechanically strong and environmentally stable. Early attempts utiliseddehydrohalogenation or Wittig condensation reactions which resulted in the formation of intractable oligomeric powders. TheWessling-Zimmermann precursor is a water-soluble PPV prepolymer (cf. Durham route) which allows the reproducibleformation of high molecular weight free standing films.PPVs were originally synthesised via the popular Gilch route which uses the bis(chloromethyl)benzene precursor monomer inTHF in the presence of t-butoxide as non-nucleophilic base. The reaction leads to a rather il-defined product with limitedconjugation length and defects along the polymer backbone. The precursor sulfonium electrolyte is prepared in aqueoussolution (Wessling route to PPV, less defects, longer conjugation, milder) by the base induced polymerisation of theappropriate bis-sulfonium monomer. The polymerisation is quenched by addition of dilute acid and the reaction mixture isthen dialysed against water to separate the high molecular weight fraction as well as the sodium and chloride ions. A study ofthe polymerisation mechanism revealed the existence of a quinoid intermediate during the early stages of the polymerisation.An alternative radical mechanism has been considered but ruled out by the experimental evidence. Na Cl Cl R R R Cl S S NaOH S Cl S S R R Cl R Cl R R R (i) dialysis n Nu S n (ii) H + / heat S R R Cl R
An interesting group of electron-deficient PPVs are the cyano substituted PPVs which are prepared by a Knoevenagelcondensation reaction between an aromatic diacetonitrile and an aromatic dialdehyde.The versatiliy of the Knoevenagel condensation reaction renders this route suitable for the synthesis of heteroaromaticcyanopolymers including well-defined alternating copolymers. As always important in the context of conducting polymers isthe ability to influence the bandgap in a molecular predictable fashion so that their electronic properties can be tuned andtailored according to the desired application.2.6. OligomersHow planar is a PPV molecule? Drawn PPV films were analysed by X-ray diffraction and NMR. The results demonstratedthat the average tilt of the phenylene ring relative to the chain axis was 7.7o, close but not exactly equal to the 9.2o predictedfor a trans-stilbene-like structure. Highly oriented PPV shows high electrical conductivity upon vapour-phase doping withAsF5 but iodine doped films show only modest conductivities.PPV oligomers have been synthesised by the Wittig reaction in order to obtain model compounds for physical characterisationstudies aimed at a more detailed understanding of the conduction mechanism present in doped conjugated polymers. Br CH2 P(Ph)3 LiOEt / EtOH DMF / RT NBS PPh3 CCl4 / 80oC toluene / 110 oC OHC CHO It is a challenge to prepare PS oligomers!!!2.7. Ladderpolymers2.8. Poly(thiophene)sHeteroaromatic polyarylenes can be prepared employing similar synthetic strategies as those described for poly(phenylene)sand poly(phenylene vinylene)s. Not only has the heteroatom an influence on the chemical and physical properties of thepolymeric product, it also has to be taken into account when preparing the required monomer (cf. aromatic heterocycleslectures).Polythiophene like many other linear polyaromatic compounds is insoluble in organic solvents (rigid backbone) andsubstitution in the 3 and/or 4 position is necessary to render the polymer soluble.With the introduction of 3-substituents, a number of different regioisomers are possible. These are head-to-head, tail-to-tailand head-to-tail. and random configurations. The issue of regioregularity pervades all of polymer chemistry and is presenteven in simple linear polymers such as polystyrene and poly(methyl methacrylate). Potentially any α-olefin is prone topolymerise to yield all of these regiochemical variations. Thus it is a significant challenge to find polymerisation reactionsand/or reaction conditions to allow to control the sequence of regioisomers at will.Studies on regioregular poly(thiophene)s, that have become accessible recently via a number of elegant routs, have shown thatcrystallinity increases with stereoregularity and that the possibility of sidechain crystallinity is essential for the development ofoptimal properties. For regiorandom polymers the optimal chain length for properties like conductivity and optical non-linearities has been determined to be in the range of 7-9. In contrast doped regioregular 3-substituted poly(thiophene) reaches
its optimal conductivity (1000 S/cm) with an dodecyl sidechain (octyl for the regiorandom polymer (20 S/cm)). 3,4-disubstitution reduces conductivity in the case of methylene groups (loss of coplanarity) because of steric hindrance. This canbe overcome by substituting the methylene group with an oxygen.McCullough’s route to regioregular poly(thiophene)s (98% HT; 70%). R LDA / THF MgBr 2 OEt 2 NiCl2(dppp) R -78-(-40 oC) -60-(-5oC) -5-25oC S Br S n head-to-tail R R R R R R S S S S S S S S S S S S R R R R R R R R R S S S S S S R R R
Solid-state UV–vis absorption spectra for films of poly(3-hexylthiophenes) with different regioregularity: (a) HT>89.5%; (b) HT:HH=70:30; (c)HT:HH=65:53; (d) HT:HH=50:50.Oxidative coupling to poly(thiophene)s using FeCl3 has also been shown to produce regioregular polymers with up to 94%HT.An interesting and intriguing property of substituted poly(thiophene)s is the temperature dependence of the UV absorption.An increase in temperature causes the λmax to shift to shorter wavelengths. This thermochromism arises from theconformational change in the aromatic backbone as a result of an increased disorder of the alkyl sidechains. Two distinctstructures are possible depending on solvent and temperature; a predominantly coplanar structure in an aggregated form in apoor solvent (or low temperatures) and a conformationally disordered non-planar structure in a good solvent (hightemperature). conductivity solution solid state regioregular 1000 S/cm 450 nm 526 nm regiorandom 20 S/cm 436 nm 480 nm S S S S S S S S S S S S S S S S S S S SElectrochemical polymerisation of thiophene is used as a convenient route to prepare thin conducting films with controlledfilm thickness. The proposed polymerisation mechanism is proposed to include a dication of two thiophene rings.
- e- S S - e- - 2H+ S S - e- - 2H+ S S H S S S S S S nThe synthesis of poly(pyrrole)s is very much related to that of poly(thiophene)s. However there is one distinct difference andthat is the reactive nitrogen-hydrogen bond. Thus protection of the amine is required to prevent sidereactions such ascrosslinking to occur. As in so many cases in polymer chemistry the t-Boc group serves well as stable protecting group whichsubsequently can be removed easily through acidic or thermal deprotection.2.9. Poly(pyrrole)sPoly(pyrrole) prepared by the Stille coupling/thermolysis sequence. (Boc) 2O NBS ClSn(CH 3)3 Pd(0) heat N N N N H n H n Boc Boc2.9.1. Stille Coupling(as an example for a variety of cross-coupling chemistries; Suzuki, Shonganishira, Yamamoto, Heck))Stille coupling. Catalytic cycle. R-R PdLn RX L (n-2) L L R Pd L R PdX R L RSnR3 L R PdR L XSnR32.10. Poly(aniline)sOxidation of aniline is the most widely employed synthetic route to polyaniline and can be performed either electrochemicallyor chemically. The reaction is usually carried out in acidic medium with a chemical oxidising agents such asammoniumpersulfate. Branching or even crosslinking during polymerisation occurs through the formation of radicals at the 2and 6 position.
NH2 - e- - 2H+ NH2 N NH2 H Cu(I) H Cu(II) NH2 Cu(II) - e- Cu(I) H - H+ NH2 NH2 - 2H+ N N NH2 H HPolyaniline can occur in a number of well-defined oxidation states. The different states range from the fully reducedleucoemeraldine via protoemeraldine, emeraldine and nigraniline to the fully oxidised pernigraniline. Unlike most otherpolyaromatics, the fully oxidised state in polyaniline is not conducting as are all the others too!. Polyaniline becomesconducting when the moderately oxidised states, in particular the emeraldine base, are protonated and charge carriers aregenerated. It is this process, generally called protonic acid doping, which makes polyaniline so unique. No electrons have tobe added or removed from the insulating material to make it conducting. N N N N N N N N H H H H N N N N N N N N emeraldine H H H H H H H Hleucoemeraldine SO3 H N N N N N N N N H H H H H H H H H H N N N N N N N Nprotoemeraldine H H H H H H H H SO3 SO3 SO3 SO3 SO3 SO3 SO3 SO3 N N N N N N N N H H H Hemeraldine N N N N N N N N H Hnigraniline N N N N N N N Npernigraniline solubleThe different oxidation states of polyaniline can also be generated by doping with oxidants such as iodine but the resultingconductivity is lower than that obtained via protonic acid doping. The conduction mechanism is believed to involve polarons.In the case of the protonated emeraldine a delocalised poly(semiquinone radical cation) is the polaronic carrier.The conductivity is affected by the water content. Completely dry samples are five times less conductive than samplescontaining some water.Self-doped polyaniline, containing sulphonic acid substituents has been synthesised by sulphonation of the emeraldine base.A different approach to the production of polyaniline (instead of long alkyl sidechain e.g.) is the use of n-alkyl sulphonic acidsas proton donor (and ionically anchored aliphatic sidechains).Stable thin films of polyaniline that can be processed out of solution are prepared from the emeraldine base withcamphorsulphonic acid as dopant. m-Cresol as cosolvent is essential to obtain a chiral crystalline structure.